Item 342. Permeable Friction Course (PFC). Typical Use. Used on high speed roadways (> 45 mph posted speed) Used to optimize safety and comfort. Typical Use. Most PFC contains PG76-xx & Fibers Asphalt Rubber (A-R) PFC used: On Concrete Pavement
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Permeable Friction Course
(> 45 mph posted speed)
On Concrete Pavement
Where a high degree of noise reduction
When it is placed on a roadway with a
high amount of cracking.
Drains better than A-R PFC
Is quieter than PFC with Fibers
110 #/sy.in. for dense graded mix
There are three PFC videos on the CD
No Penalty/Bonus provisions
More requirements for QC testing by
the Contractor and QA testing by the
342.1. Description.Construct asurface coursecomposed of a compacted permeable mixture of aggregate, asphalt binder, and additives mixed hot in a mixing plant
A. Aggregate. Furnish aggregates from sources that conform to the requirements shown in Table 1, and as specified in this Section, unless otherwise shown on the plans. Provide aggregate stockpiles that meet the definition in this Section for coarse aggregate. Do not use fine aggregate or reclaimed asphalt pavement (RAP) in PFC mixtures. Supply mechanically crushed gravel or stone aggregates that meet the definitions in Tex‑100‑E. The Engineer will designate the plant or the quarry as the sampling location. Samples must be from materials produced for the project. The Engineer will establish the surface aggregate classification (SAC) and perform Los Angeles abrasion, magnesium sulfate soundness, and Micro-Deval tests. Perform all other aggregate quality tests listed in Table 1.
Coarse Aggregate Quality Requirements
2. RAP.Do not use RAP in PFC mixtures.
B. Baghouse Fines. Fines collected by the baghouse or other dust collecting equipment may be reintroduced into the mixing drum
C. Asphalt Binder.Furnish performance-graded (PG) asphalt binder and fibers unless the plans specify asphalt-rubber (A‑R) binder. Provide asphalt binder that meets requirements of Item 300, “Asphalts, Oils, and Emulsions.”
2. A‑R BinderWhen A‑R binder is specified, provide A‑R binder that meets the Type I or Type II requirements of Section 300.2.I, “Asphalt-Rubber Binders,” unless otherwise shown on the plans. Use at least 15.0% by weight of Crumb Rubber Modifier (CRM) that meets the Grade B or Grade C requirements of Section 300.2.G, “Crumb Rubber Modifier,” unless otherwise shown on the plans.
D. Additives.When shown on the plans, use the type and rate of additive specified. Other additives that facilitate mixing or improve the quality of the mixture may be allowed when approved.
2. Lime Mineral Filler.When PG binder is specified, add lime as mineral filler at a rate of 1.0% by weight of the total dry aggregate. Do not add lime directly into the mixing drum of any plant where lime is removed through the exhaust stream unless the plant has a baghouse or dust collection system that reintroduces the lime back into the drum.
3. Antistripping Agents. If lime or a liquid antistripping agent is used, add in accordance with Item 301, “Asphalt Antistripping Agents.” When the plans require lime to be added as an antistripping agent, lime added as mineral filler will count towards the total quantity of lime specified.
342.2 Construction. Produce, haul, place, and compact the specified paving mixture. When shown on the plans, schedule and participate in a prepaving meeting with the Engineer as required in the Quality Control Plan (QCP).
A. Certification. Personnel certified by the Department-approved hot-mix asphalt certification program must conduct all mixture designs, sampling, and testing in accordance with Table 2. In addition to meeting the certification requirements in Table 2, all Level II certified specialists must successfully complete an approved Superpave training course. Supply the Engineer……
Test Methods, Test Responsibility, and Minimum Certification Levels
B. Reporting.Use Department-provided software to record and calculate all test data. The Engineer and the Contractor shall provide any available test results to the other party when requested. The Engineer and the Contractor shall immediately report to the other party any test result that requires production to be suspended or fails to meet the specification requirements. Use the approved communication method (e.g., email, diskette, hard copy) to submit test results to the Engineer.
When directed, use the procedures described in Tex‑233‑F to plot the results of all productions and placement testing. Update the control charts as soon as test results for each sublot become available. Make the control charts readily accessible at the field laboratory. The Engineer may suspend production for failure to update control charts.
C. QCP. Develop and follow the QCP in detail. Obtain approval from the Engineer for changes to the QCP made during the project. The Engineer may suspend operations if the Contractor fails to comply with the QCP.
When directed, submit a written QCP to the Engineer before the mandatory prepaving meeting. Receive the Engineer’s approval of the QCP before beginning production. Include the following items in the QCP
D. Mixture Design.Unless otherwise shown on the plans, use the PFC design procedure given in Tex-204-F, Part V, to design a mixture meeting the requirements listed in Tables 1,3, and 4. Use Ndes= 50 as the design number of gyrations.
The Contractor may submit a new mixture design at anytime during the project. The Engineer will approve all mixture designs before the Contractor can begin production. When shown on the plans, the Engineer will provide the mixture design.
Provide the Engineer with a mixture design report using Department‑provided software. Include the following items in the report:
Master Gradation Band (% Passing by Weight or Volume) and Binder Content
Laboratory Mixture Design Properties
Testing Frequency and Mixture Production Tolerances
2. JMF Adjustments. Produce the mixture within the operational tolerances listed in Table 5. The Engineer may suspend production if corrective actions are not taken when operational tolerances are exceeded. With approval from the Engineer, the JMF target values may be adjusted as needed. Document any changes to the JMF with a subsequent JMF number. The Engineer may adjust the target asphalt percentage or fiber percentage within the operational tolerances of the JMF.
E. Production Operations.Perform a new trial batch when the plant or plant location is changed. Perform QC at the frequency and within the tolerances of Table 5……
At any time during production the Engineer may require the Contractor to verify the following based on quantities used:
• lime content (within ±0.1% of JMF), when PG binder is specified;
• fiber content (within ±0.03% of JMF), when PG binder is specified; and
•CRM content (within ±1.5% of JMF), when A‑R binder is specified.
When A‑R binder is specified, maintain the in-line measuring device to verify the A‑R binder viscosity of at least 2,500 centipoise at 350°F unless otherwise approved.
3. Lay-Down Operations.Measure the temperature of mixture delivered to the paver and take corrective action if needed to ensure the temperature does not drop below 280°F.For each sublotuse a handheld infrared thermometer to obtain a thermal profile of the uncompacted mat immediately behind the paver.
Record the information on Department QC/QA forms and submit the forms to the Engineer.
a. Thermal Profile.For each sublot, obtain a thermal profile using Tex‑244‑F.The Engineer may reduce the testing frequency based on a satisfactory test history. The Engineer may also obtain as many thermal profiles as deemed necessary.If the temperature differential is greater than 25°F, the area will be deemed to have thermal segregation.Take corrective action to eliminate areas that have thermal segregation.Unless otherwise directed,suspend operations if maximum temperature differential exceeds 50°F. Resume operations when the Engineer determines that subsequent production will meet the requirements of this Item.
Note: If thermal segregation exists, the contractor has to take corrective action
(density profile not required).
H. Compaction.Roll the freshly placed PFC with a steel-wheeled roller, operated in static mode, to seat the mixture without excessive breakage of the aggregate and to provide a smooth surface and uniform texture. Do not use pneumatic rollers. Thoroughly moisten the roller drums with a soap-and-water solution to prevent adhesion. Unless otherwise directed, use only water or an approved release agent on rollers, tamps, and other compaction equipment
The Engineer may use or require the Contractor to use Tex‑246‑F to test and verify that the compacted mixture has adequate permeability. Adjust the mixture design or construction methods if the compacted mixture does not exhibit adequate permeability.
Note: The permeability test should be performed the first day of placement to verify that the mix is not over compacted. (Video on CD)
I. Acceptance Plan. Sample and test the hot mix on a lot and sublot basis. A production lot consists of 4 equal sublots. Lot 1 will be 1000 tons. The Engineer will select subsequent lot sizes based on the anticipated daily production. The lot size will be between 1,000 and 4,000 tons. The Engineer may change the lot size before the Contractor begins any lot. If the production or placement test results are not within the acceptable tolerances listed in Table 5, suspend production until test results or other information indicated to the satisfaction of the Engineer that the next material produced or placed will meet the specified values.
3. Operational Tolerances.Control the production process within the operational tolerances listed in Table 5.When production is suspended, the Engineer will allow production to resume when test results or other information indicates the next mixture produced will be within the operational tolerances.
342.5 Measurement.PFC will be measured by the ton of composite PFC. The composite PFC is defined as the asphalt, aggregate, and additives.The weights of asphalt and aggregate will be calculated based on the measured weight of PFC and the target percentage of asphalt and aggregate. Measure the weight on scales in accordance with Item 520, “Weighing and Measuring Equipment.”
A. Asphalt. The asphalt weight in tons will be determined from the total weight of PFC. Measured asphalt percentage will be obtained using Tex‑236‑F or asphalt flow meter readings, as determined by the Engineer.
Caution: If you use an ignition oven, make sure that you account for the % fibers used. Flow meter readings are preferred especially if you are using A-R binder.
2. Measured Percentage.The measured asphalt percentage will be used for payment for that lot’s productionwhen the measured percentage is more than 0.3 percentage points below the JMF target asphalt percentage.
B. Aggregate. The aggregate weight in tons will be determined from the total weight of PFC less the weight of the asphalt.
342.6 Payment. The work performed and materials furnished in accordance with this Item and measured as provided under “Measurement” will be paid for at the unit price bid for “PFC (Asphalt)” of the binder specified and for “PFC (Aggregate)” of the grade and surface aggregate classification specified. These prices are full compensation for surface preparation, materials including tack coat, placement, equipment, labor, tools, and incidentals.
Trial batches will not be paid for unless they are included in pavement work approved by the Department.
Pay adjustment for ride quality will be determined in accordance with Item 585, “Ride Quality for Pavement Surfaces.”
Note: There are no bonus or penalty provisions.